pubs.acs.org/Langmuir © 2009 American Chemical Society
A Facile and Controllable Strategy to Synthesize Au-Ag Alloy Nanoparticles within Polyelectrolyte Multilayer Nanoreactors upon Thermal Reduction Li Shang, Lihua Jin, Shaojun Guo, Junfeng Zhai, and Shaojun Dong* State Key Laboratory of Electroanalytical Chemistry, Changchun Institute of Applied Chemistry, Graduate School of the Chinese Academy of Sciences, Chinese Academy of Sciences, Changchun, 130022, China Received October 26, 2009. Revised Manuscript Received November 27, 2009 A new synthesis strategy has been developed for the preparation of bimetallic gold-silver (Au-Ag) alloy nanoparticles by the virtue of polyelectrolyte multilayer (PEM) nanoreactors. By controlling the assembly conditions, gold and silver ions can be effectively loaded onto the PEM composed of polyethylenimine (PEI) and poly(acrylic acid) (PAA) simultaneously. Upon further thermal treatment, Au-Ag alloy nanoparticles with sizes of ca. 3.8 nm formed in the PEM, which were characterized in detail by UV-vis absorption spectroscopy, transmission electron microscopy (TEM), X-ray photoelectron spectroscopy (XPS), X-ray diffraction (XRD), and energy-dispersive X-ray (EDX) analysis. Appearance of a single plasmon band in the visible region and lack of apparent core-shell structures in the TEM images confirm the formation of homogeneous Au-Ag alloy nanoparticles. In addition, the surface plasmon absorption band of the Au-Ag alloy nanoparticles shows linear blue-shift with increasing Ag content, which also supported the formation of alloy nanoparticles. Several key parameters of the present strategy have been investigated, which showed that pH of both the assembly solution and gold salt solution and the choice of polymers for constructing PEM, as well as the reduction approach, all played an important role in successfully synthesizing bimetallic Au-Ag nanoparticles. The formation mechanism of alloy nanoparticles has also been discussed based on the spectral evolution during the thermal reduction.
Introduction Nanomaterials are at the leading edge of the rapidly developing field of nanotechnology.1 The development of reliable experimental strategies for synthesizing nanomaterials with well-controlled composition, high monodispersity, and multifunction is one of the challenging themes in current nanotechnology.2 Metal particles in the nanometer size regime show distinct size-dependent properties than those of bulk metals, which led to extensive investigations involving metal nanoparticles, especially gold/silver, as building blocks for nanoscale materials and devices in the last 2 decades.3 Recently, bimetallic nanoparticles with either alloyed or core-shell structures have gained significant interest due to new properties that arise from the combination of different compositions of metals on the nanoscale.4 In particular, the properties of these bimetallic particles can be facilely tailored by the composition besides the usual size and shape manipulation. Their unique *To whom correspondence should be addressed. Fax: þ86-431-85689711. E-mail: [email protected]
. (1) (a) Roduner, E. Chem. Soc. Rev. 2006, 35, 583. (b) Zhao, Y.; Fu, H.; Peng, A.; Ma, Y.; Xiao, D.; Yao, J. Adv. Mater. 2008, 20, 2859. (c) Service, R. F. Science 2008, 321, 1036. (d) Zhang, L. J.; Webster, T. J. Nano Today 2009, 4, 66. (2) (a) Perro, A.; Reculusa, S.; Ravaine, S.; Bourgeat-Lami, E.; Duguet, E. J. Mater. Chem. 2005, 15, 3745. (b) Park, J.; Joo, J.; Kwon, S. G.; Jang, Y.; Hyeon, T. Angew. Chem., Int. Ed. 2007, 46, 4630. (c) Berti, L.; Burley, G. A. Nat. Nanotechnol. 2008, 3, 81. (3) (a) Shenhar, R.; Rotello, V. M. Acc. Chem. Res. 2003, 36, 549. (b) Liao, H. W.; Nehl, C. L.; Hafner, J. H. Nanomedicine 2006, 1, 201. (c) Baron, R.; Willner, B.; Willner, I. Chem. Commun. 2007, 323. (d) Lee, J. S.; Kim, Y. M.; Kwon, J. H.; Shin, H.; Sohn, B. H.; Lee, J. Adv. Mater. 2009, 21, 178. (4) (a) Ferrando, R.; Jellinek, J.; Johnston, R. L. Chem. Rev. 2008, 108, 845. (b) Major, K. J.; De, C.; Obare, S. O. Plasmonics 2009, 4, 61. (5) Nishida, N.; Shiraishi, Y.; Kobayashi, S.; Toshima, N. J. Phys. Chem. C 2008, 112, 20284. (6) (a) Hunyadi, S. E.; Murphy, C. J. J. Mater. Chem. 2006, 16, 3929. (b) Sharma, A. K.; Gupta, B. D. Nanotechnology 2006, 17, 124. (c) Zou, X.; Ying, E.; Dong, S. J. Colloid Interface Sci. 2007, 306, 307.
Langmuir 2010, 26(9), 6713–6719
properties have been utilized in electronic5 and optical6 as well as catalysis applications,7 which proves to be more effective than monometallic nanocrystals. For example, one recent study indicated that bimetallic Au-Ag nanoparticles displayed considerably more sensitivity in SERS analysis as biosensors than individual components.8 A number of synthetic strategies have been developed for the preparation of bimetallic nanoparticles, including wet chemical approach,9 photochemical method,10 electroless plating,11 electrochemical synthesis,12 and thermal reduction.13 However, most previous studies have been carried out in liquid mixtures or solutions.9-12 In many cases, in order to manipulate and process these nanoparticles for practical applications such as optoelectronics and sensor devices, they have to be embedded within polymer matrixes, or on solid substrates.6b,13a,14 Although bimetallic nanoparticles which are presynthesized in solution can be (7) (a) Li, X.; Li, B.; Cheng, M.; Du, Y.; Wang, X.; Yang, P. J. Mol. Catal. A: Chem. 2008, 284, 1. (b) Huang, J.; Vongehr, S.; Tang, S.; Lu, H.; Shen, J.; Meng, X. Langmuir 2009, 25, 11890–11896. (8) Liu, Y. C.; Yu, C. C.; Hsu, T. C. Electrochem. Commun. 2007, 9, 639. (9) (a) Link, S.; Wang, Z. L.; El-Sayed, M. A. J. Phys. Chem. B 1999, 103, 3529. (b) Mallin, M. P.; Murphy, C. J. Nano Lett. 2002, 2, 1235. (c) Kariuki, N. N.; Luo, J.; Maye, M. M.; Hassan, S. A.; Menard, T.; Naslund, H. R.; Lin, Y.; Wang, C.; Engelhard, M. H.; Zhong, C. J. Langmuir 2004, 20, 11240. (d) Rodriguez-Gonzalez, B.; Burrows, A.; Watanabe, M.; Kiely, C. J.; Marzan, L. M. L. J. Mater. Chem. 2005, 15, 1755. (e) Raveendran, P.; Fua, J.; Wallen, S. L. Green Chem. 2006, 8, 34. (10) (a) Peng, Z.; Spliethoff, B.; Tesche, B.; Walther, T.; Kleinermanns, K. J. Phys. Chem. B 2006, 110, 2549. (b) Gonzalez, C. M.; Liu, Y.; Scaiano, J. C. J. Phys. Chem. C 2009, 113, 11861. (11) (a) Zhang, Q.; Xie, J.; Liang, J.; Lee, J. Y. Adv. Funct. Mater. 2009, 19, 1387. (b) Wang, C.; Peng, S.; Chan, R.; Sun, S. Small 2009, 5, 567. (12) (a) Zhou, M.; Chen, S.; Zhao, S.; Ma, H. Physica E 2006, 33, 28. (b) Alqudami., A.; Annapoorni, S.; Shivaprasad, G. S. M. J. Nanopart. Res. 2008, 10, 1027. (13) (a) Pal, S.; De, G. Chem. Mater. 2005, 17, 6161. (b) Prvulescu, V. I.; Prvulescu, V.; Endruschat, U.; Filoti, G.; Wagner, F. E.; Kubel, C.; Richards, R. Chem.;Eur. J. 2006, 12, 2343. (c) Som, T.; Karmakar, B. Nano Res. 2009, 2, 607.
Published on Web 12/17/2009
Shang et al.
in the fields including optical devices, heterogeneous catalysis, and biomedical research.5,6,7b,14 The principle of our strategy is schematically shown in Figure 1. In general, multilayer films via layer-by-layer deposition of polyethylenimine (PEI) and poly(acrylic acid) (PAA) are fabricated first. Then AuCl4- and Agþ are incorporated into the assembled PEM films sequentially via the interaction between the polyelectrolytes and the metal ions. Upon further thermal reduction, Au-Ag alloy nanoparticles are formed within PEM films. The present protocol is simple and controllable, which can be easily extended to synthesize other bimetallic or multicomponent nanoparticles.
Experimental Section Figure 1. Schematic of the PEM buildup and subsequent reduction process.
further deposited on a support, their original structure, size, and morphology are hardly retained.14b Moreover, it would be more favorable to combine the synthesis and immobilization of nanoparticles within one step, which suggests the importance and urgency to develop an in situ synthesis strategy of bimetallic nanoparticles within the films or other support. Recently, polyelectrolyte multilayer (PEM) films, constructed through the electrostatic layer-by-layer self-assembly of oppositely charged polyelectrolytes, is of great interest as a facile means for creating functional nanomaterials.15 These PEM are promising nanoreactors which have been applied for synthesizing a broad range of nanomaterials, because the multilayer films can be facilely tuned with desired composition and thickness, deposited onto different substrates with predetermined morphologies, and easily removed after nanomaterials synthesis.15a Many groups including us have reported the successful synthesis of monometallic nanoparticles (such as Au, Ag, and Pt) within PEM,16 which demonstrated its great potential for synthesizing nanoparticles in a simple and controllable approach. Herein, we further extended the utilization of PEM to synthesize bimetallic alloy nanoparticles. To the best of our knowledge, this is the first report of preparing bimetallic nanoparticles by the virtue of PEM nanoreactors. As an example of this strategy, we will report the synthesis of Au-Ag alloy nanoparticles within the PEM composed of weak polyelectrolytes. The Au-Ag bimetallic system was chosen based on the following reasons. First, Au and Ag are known to have very similar lattice constants and are completely miscible in all proportions, forming homogeneous alloys in bulk phases.17 Second, Au-Ag nanoparticles show interesting optical properties and the plasmon absorption band depends on the alloy composition.9b,18 Third, Au-Ag alloy nanoparticles combine both merits of Au and Ag, which leads to their promising application (14) (a) Ong, B. H.; Yuan, X. C.; Tjin, S. C. Fiber Integr. Opt. 2007, 26, 229. (b) Liu, X.; Wang, A.; Yang, X.; Zhang, T.; Mou, C.; Su, D.; Li, J. Chem. Mater. 2009, 21, 410. (15) (a) Shi, X.; Shen, M.; Mohwald, H. Prog. Polym. Sci. 2004, 29, 987. (b) Srivastava, S.; Kotov, N. A. Acc. Chem. Res. 2008, 41, 1831. (c) Wang, Y.; Angelatos, A. S.; Caruso, F. Chem. Mater. 2008, 20, 848. (16) (a) Xiong, H.; Cheng, M.; Zhou, Z.; Zhang, X.; Shen, J. Adv. Mater. 1998, 10, 529. (b) Dai, J.; Bruening, M. L. Nano Lett. 2002, 2, 497. (c) Wang, T. C.; Rubner, M. F.; Cohen, R. E. Langmuir 2002, 18, 3370. (d) Chen, H.; Dong, S. Talanta 2007, 71, 1752. (e) Shang, L.; Wang, Y.; Huang, L.; Dong, S. Langmuir 2007, 23, 7738. (f) Chia, K. K.; Cohen, R. E.; Rubner, M. F. Chem. Mater. 2008, 20, 6756. (f) Kgoo, H. Y.; Choi, W. S.; Park, J. H.; Kim, D. Y. Macromol. Rapid Commun. 2008, 29, 520. (h) Zan, X.; Su, Z. Langmuir 2009, 25, 12355–12360. (17) Okamoto, H.; Massalski, T. B. Phase Diagrams of Binary Gold Alloys; ASM International: Metals Park, OH, 1987. (18) Senapati, S.; Ahmad, A.; Khan, M. I.; Sastry, M.; Kumar, R. Small 2005, 1, 517.
6714 DOI: 10.1021/la9040612
Reagents. Branched polyethylenimine (PEI, Mw = 25000), linear polyethylenimine (LPEI, Mn = 423), Poly(methacrylic acid) (PMAA, Mw = 9500), poly(diallyldimethylammonium chloride) (PDDA, Mw = 20000), and poly(sodium styrenesulfonate) (PSS, Mw = 70000) were purchased from Sigma-Aldrich. Poly(acrylic acid) (PAA, Mw = 240000) was bought from Alfa Aesar. Hydrogen tetrachloroaurate (HAuCl4 3 3H2O) and AgNO3 were purchased from Beijing Chemical Co. (China). All reagents were of analytical reagent grade, and used as received. Indium-tin oxide (ITO) covered glass plates were purchased form Shenzhen Hivac Vacuum Photoelectronics Co. Ltd. (China, resistivity 2.0, the binding ability of PEM toward gold complex ions would decrease with increasing pH, because less amine groups that are capable of binding gold ions were available (seen in Figure S1 in the Supporting Information).16f Therefore, we adopted a HAuCl4 solution with pH 2.0 for loading gold ions into the film. To probe other factors responsible for the synthesis of bimetallic Au-Ag alloy nanoparticles in the present approach, we also conducted other control experiments. First, we performed the same preparation by changing either or both PEI/PAA with other common polyelectrolytes such as PDDA, PSS, LPEI and PMAA. The results showed that PEM composed of (PDDA/PSS)n, (PDDA/PAA)n, or (PEI/PSS)n all failed in synthesizing bimetallic nanoparticles. In contrary, PEM composed of (LPEI/PAA)n, (PEI/PMAA)n, or (LPEI/PMAA)n could obtain similar alloy nanoparticles at suitable assembly conditions. These results clearly suggested the importance of coexisting amine groups and carboxylic groups in the PEM films, which accorded with our notion that both groups were necessary for adsorbing metal ions. Second, we attempted to reduce metal ions by other approaches rather than thermal treatment. While reduction by immersing metal ions-containing PEM films in the NaBH4 (0.01 M) could proceed very fast within 10 min and form alloy nanoparticles, the resultant film was found to exhibit poor stability, which was possibly caused by the harsh reaction conditions. Photoreduction by radiating the film with a UV lamp at 365 nm could also result in the production of bimetallic nanoparticles, but the reaction proceeded too slowly (longer than 24 h). Therefore, thermal reduction was adopted in our experiment. Mechanism for Alloy Formation. We then try to probe the possible formation mechanism of alloy nanoparticles in our system. Since gold and silver have similar lattice constants and can form homogeneous alloys in bulk phases, the formation of alloy nanoparticles was actually not unexpected for PEM incorporated with both Au and Ag ions in the films. On the basis of the evolution of absorption spectra of PEM upon thermal reduction as shown in Figure 4, we speculated the possible alloy formation processes as following. When the metal ions-loaded films were subjected to heating at 473 K, gold ions in the film will first be reduced to form small clusters due to its redox advantage over silver.6a,27 During this process, the plasmon absorption will be dominated by the SPR of gold. Further heating will cause the nearby Ag ions being coreduced along with gold ions on the surface of small gold clusters, and the plasmon band will blue-shift correspondingly due to the doping of Ag within the particles. With extending the heating time, alloy nanoparticles will grow gradually until they reach a size with a surface area that can be stabilized by the surrounding polymers. Moreover, previous studies indicated that high concentration of metal ions within the films could also favor alloying of metal nanoparticles.31 Although the detailed growth mechanism of alloy nanoparticle is not well understood at present, the formation of alloy nanoparticles (31) Roy, R. K.; Mandal, S. K.; Pal, A. K. Eur. Phys. J. B 2003, 33, 109.
6718 DOI: 10.1021/la9040612
Shang et al.
can be well supported by our experimental results. The spectral evidence came from the appearance of a single plasmon band in the visible range as shown in Figure 4 and the linear blue-shift in the plasmon peak with the increase in Ag/Au ratio (Figure 5). Also the lack of apparent core-shell structures in the TEM images (Figure 6) and homogeneous Au/Ag distribution throughout the film by EDX analysis further supported the formation of gold-silver alloy nanoparticles. Merits of the Strategy. Compared with previous methods for synthesizing Au-Ag alloy nanoparticles, the present strategy by utilizing PEM nanoreactors possesses several distinct advantages: (a) The structure and composition of PEM are variable and tunable via the choice of polyelectrolytes, which allows the facile introduction of additional function/property into the films accompanying with the formation of alloy nanoparticles.15a For example, the choice of polymers with electroactive groups is expected to endow the resultant nanostructured films with electroactive property. Moreover, the strategy of PEM nanoreactors is favorable for synthesizing ultrasmall nanoparticles due to the restricting effect of surrounding polyelectrolytes to the growth of nanoparticles, such as Au-Ag alloy particles with sizes of ca. 3.8 nm in our case. Previous studies indicated that these small-sized metal nanoparticles showed particularly high reactivities, which was favorable for their catalytic applications.14b (b) The concentration, composition, and optical properties of the nanoparticles in the film could be readily tuned by manipulating the multilayer processing conditions. As shown in Figure 5, while the Ag/Au ratio can be controlled by controlling the immersing time in AgNO3, the optical properties of the nanostructured films can be changed correspondingly. This suggested the feasibility of modulating the optical properties of the film. In addition, the concentration and size of metal nanoparticles in the films can also be facilely controlled by tuning the assembly conditions such as metal salt concentration, pH, and bilayer number. As an example, absorption spectra of PEM with different bilayer numbers (n = 1-7) after loading metal ions and subjected to thermal reduction were investigated (seen in Figure S2 in the Supporting Information). The results showed that the absorbance of formed alloy nanoparticles increased gradually and exponentially with increasing the bilayer numbers, which accorded well with the result in Figure 2 that the (PEI/PAA)n film grows in an exponential mode. The results herein also suggested the feasibility of tuning the density of nanoparticles in the film in a facile approach. (c) The resultant alloy nanoparticles-embedded films were found to exhibit good chemical stability, as evidenced by negligible spectral changes after aging the film in the air for over 1 month. We attributed this stability to the following two reasons. On one hand, since the alloy nanoparticles were in situ formed within multilayer films, due to the association of metal with the component of the film, movement of the formed nanoparticles was restricted and hence improved the stability of the resulting film.16e On the other hand, previous studies indicated that reduction of metal ions by heating could result in the cross-linking of PEI/PAA systems via heat-induced amide formation from carboxylate-ammonium complexes,16b which could also strengthen the film. (d) Finally, the present strategy can be extended to prepare other bimetallic or multicomponent nanoparticles within PEM nanoreactors, provided the assembling polyelectrolytes possess necessary binding groups for the respective metal ions. In addition, this method can be applicable to synthesize bimetallic nanoparticles on either planar or curve surfaces, for example, Langmuir 2010, 26(9), 6713–6719
Shang et al.
on the surface of colloid particles, which can further extend the application of formed nanoparticles.
Conclusions In summary, we have reported a general strategy of synthesizing small-sized, composition-controllable Au-Ag alloy nanoparticles within PEM nanoreactors. By controlling assembly conditions, gold and silver ions can be effectively incorporated into PEM of (PEI/PAA)n. Upon further thermal reduction, alloy nanoparticles can be obtained, which is confirmed by both absorption spectroscopy and TEM results. The concentration and composition of nanoparticles, the component and optical properties of the film can all be readily tuned by controlling the experimental conditions. This work not only presents a new strategy of preparing Au-Ag alloy nanoparticles, but also extends the applicability of PEM nanoreactors from synthesizing monometallic nanoparticles to bimetallic nanoparticles.
Langmuir 2010, 26(9), 6713–6719
Moreover, such a strategy can be extended for synthesizing a wide variety of other composite nanoparticles other than the present model system (Au-Ag), which is expected to be of great importance for both synthesis and further application of these attractive nanomaterials. Acknowledgment. This work was supported by the National Natural Science Foundation of China (No. 20820102037) and the Special Funds for Major State Basic Research Projects of China (973 Project 3010CB933603). Supporting Information Available: Figures showing the absorption spectra of PEM film after immersing in the HAuCl4 solution at different pH and absorption spectra of as-prepared nanoparticles in PEM film with different bilayer numbers. This material is available free of charge via the Internet at http://pubs.acs.org.